1 introduction to polyolefins
1Introduction to Polyolefins
It is a near perfect molecule [ . . . ].Jim Pritchard, Phillips Petroleum Company
Polyolefins are used in a wide variety of applications, including grocery bags,containers, toys, adhesives, home appliances, engineering plastics, automotiveparts, medical applications, and prosthetic implants. They can be either amorphousor highly crystalline, and they behave as thermoplastics, thermoplastic elastomers,or thermosets.
Despite their usefulness, polyolefins are made of monomers composed of onlycarbon and hydrogen atoms. We are so used to these remarkable polymers thatwe do not stop and ask how materials made out of such simple units achieve thisextraordinary range of properties and applications. The answer to this questionlies in how the monomer molecules are connected in the polymer chain to definethe molecular architecture of polyolefins. By simply manipulating how ethylene,propylene, and higher α-olefins are bound in the polymer chain, polyolefins withentirely new properties can be produced.
Polyolefins can be divided into two main types, polyethylene and polypropylene,which are subdivided into several grades for different applications, as discussedlater in this chapter.1) Taking a somewhat simplistic view, three components areneeded to make a polyolefin: monomer/comonomer, catalyst/initiator system, andpolymerization reactor. We will start our discussion by taking a brief look at eachof these three components.
Commercial polyethylene resins, despite their name, are most often copoly-mers of ethylene, with varying fractions of an α-olefin comonomer. The most
1) Ethylene-propylene-diene(EPDM) terpoly-mers, another important polyolefin type,are elastomers with a wide range of ap-plications. They are made using catalystsand processes similar to those used to
produce polyethylene and polypropylene.Even though they are not discussed explic-itly in this book, several of the methodsexplained herein can be easily adopted toEPDM processes.
Polyolefin Reaction Engineering, First Edition. Joao B. P. Soares and Timothy F. L. McKenna.© 2012 Wiley-VCH Verlag GmbH & Co. KGaA. Published 2012 by Wiley-VCH Verlag GmbH & Co. KGaA.
2 1 Introduction to Polyolefins
commonly used α-olefins are 1-butene, 1-hexene, and 1-octene. They are usedto decrease the density and crystallinity of the polyolefin, changing its physicalproperties and applications. Industrial polypropylene resins are mostly isotacticmaterials, but a few syndiotactic grades are also available. There are two main typesof propylene copolymers: random propylene/ethylene copolymers2) and impactpropylene/ethylene copolymers.
At the heart of all polyolefin manufacturing processes is the system used topromote polymer chain growth. For industrial applications, polyethylene is madewith either free radical initiators or coordination catalysts, while polypropyleneis produced only with coordination catalysts. Low-density polyethylene (LDPE)is made using free radical processes and contains short chain branches (SCB)and long chain branches (LCB). Its microstructure is very different from that ofpolyethylenes made with coordination catalysts. Coordination catalysts can controlpolymer microstructure much more efficiently than free radical initiators andare used to make polyolefins with a range of properties unimaginable beforetheir discovery. The quotation at the beginning of this chapter was motivated bythe revolutionary synthesis of unbranched, linear polyethylene, the ‘‘near perfectmolecule,’’ using a Phillips catalyst.
Catalyst design is behind the success of modern industrial olefin polymerizationprocesses because the catalyst determines how the monomers will be linked inthe polymer chain, effectively defining the polymer microstructure and properties.Industrial and academic research on olefin polymerization catalysis have beenvery dynamic since the original discoveries of Ziegler and Natta (Ziegler–Nattacatalysts) and Hogan and Banks (Phillips catalysts), with many catalyst familiesbeing developed and optimized at a rapid pace. There are basically four main typesof olefin polymerization catalysts: (i) Ziegler–Natta catalysts, (ii) Phillips catalysts,(iii) metallocene catalysts, and (iv) late transition metal catalysts. Ziegler–Nattaand Phillips catalyst were discovered in the early 1950s, initiating a paradigmshift in olefin polymerization processes, while metallocene and late transitionmetal catalysts (sometimes called post-metallocenes) were developed in the 1980sand 1990s, respectively. In Chapter 3, olefin polymerization catalysts and mecha-nisms are discussed in detail, while polymerization kinetic models are developedin Chapter 5. For our purposes in this chapter, it suffices to say that polymer-ization with all coordination catalyst types involves monomer coordination to thetransition metal active site before insertion in the metal–carbon bond at oneend of the polymer chain. The coordination step is responsible for the versatil-ity of these catalysts: since the incoming monomer needs to coordinate to theactive site before propagation may occur, the electronic and steric environmentaround it can be changed to alter polymerization parameters that control thechain microstructure, such as propagation and chain transfer rates, comonomerreactivity ratios, stereoselectivity, and regioselectivity. This concept is illustrated inFigure 1.1.
2) Propylene/1-butene copolymers andpropylene/ethylene/α-olefin terpolymers
are also manufactured, but in a smallerscale.
1.1 Introduction 3
Figure 1.1 Coordination step before ethy-lene insertion on a polyethylene chain(active site control).
R* + M RM*
RM* + M RMM*
R(M)n* + M R(M)n+1*
Figure 1.2 Generic free radical polymerization(chain-end control). R∗, free radical initiator;M, monomer.
This mechanism controls the polymer microstructure better than free radicalpolymerization, where the chemical nature of the free radical initiator stops beingimportant after a few propagation steps since the polymerization locus moves awayfrom the initiator molecule, as illustrated in Figure 1.2. Free radical processes forLDPE production are not the main topic of this book and are only discussed brieflyas comparative examples.
Even though a few processes for ethylene polymerization use homogeneouscatalysts in solution reactors, most olefin polymerization processes operate withheterogeneous catalysts in two-phase or three-phase reactors. This adds an ad-ditional level of complexity to these systems since inter- and intraparticle massand heat transfer resistances during polymerization may affect the polymerizationrate and polymer microstructure. If significant, mass and energy transport limita-tions create nonuniform polymerization conditions within the catalyst particles thatlead to nonuniform polymer microstructures. Many other challenging problems areassociated with the use of heterogeneous catalysts for olefin polymerization, such ascatalyst particle breakup, agglomeration, growth, and morphological development,all of which are discussed in Chapter 7.
All the phenomena mentioned above take place in the polymerization reactor.The variety of polyolefin reactors can be surprising for someone new to the field:polyolefins are made in autoclave reactors, single- and double-loop reactors, tubularreactors, and fluidized-bed reactors; these processes may be run in solution, slurry,bulk, or gas phase. Each reactor configuration brings with it certain advantages,but it also has some disadvantages; the ability to select the proper process for agiven application is an important requirement for a polyolefin reaction engineer.Chapter 4 discusses these different reactor configurations and highlights someimportant polyolefin manufacturing processes. Reactor models that take intoaccount micromixing and macromixing effects, residence time distributions, andmass and heat transfer phenomena at the reactor level are needed to simulate theseprocesses, as explained in Chapter 8.
Catalyst type, polymerization mechanism and kinetics, inter- and intraparticlemass and heat transfer phenomena, and macroscale reactor modeling are essentialfor the design, operation, optimization, and control of polyolefin reactors. Figure 1.3
4 1 Introduction to Polyolefins
Multiple length scales High complexity
Figure 1.3 Modeling scales in polyolefin reaction engineering.
shows how these different length scales are needed to help us understand olefinpolymerization processes.
In summary, much science and technology is hidden behind the apparentsimplicity of everyday polyethylene and polypropylene consumer goods. No othersynthetic polymer is made with such a variety of catalyst types, reactor configura-tions, and microstructural complexity. In this book, we will explain how, from suchsimple monomers, polyolefins have become the dominant commodity plastic inthe twenty-first century.
Polyethylene resins are classified into three main types: LDPE, linear low-densitypolyethylene (LLDPE), and high-density polyethylene (HDPE). This traditionalclassification distinguishes each polyethylene type according to its densityrange: 0.915–0.940 g cm−3 for LDPE, 0.915–0.94 g cm−3 for LLDPE,3) and0.945–0.97 g cm−3 for HDPE, although these limits may vary slightly amongdifferent sources. Lower-density polyethylene resins (<0.915 g cm−3) aresometimes called ultra low-density polyethylene (ULDPE) or very low-densitypolyethylene (VLDPE). HDPE with molecular weight averages of several millionsis called ultrahigh molecular weight polyethylene (UHMWPE). To reduce the
3) Sometimes polyethylene resins in therange 0.926–0.940 g cm−3 are calledmedium-density polyethylene (MDPE).
1.2 Polyethylene Resins 5
LDPE LLDPE/VLDPE HDPE
0.941–0.97 g cm−30.915–0.94 g cm−3/ 0.88–0.915 g cm−30.910–0.940 g cm−3
Figure 1.4 Classification of polyethylene types according to branching structure anddensity.
number of acronyms in this book, we have often grouped MDPE, LLDPE, ULDPE,and VLDPE under the generic term LLDPE and have made no distinction betweenHDPE and UHMWPE; these resins are very similar from a structural point ofview, as explained below.
This division according to polyethylene density or molecular weight, althoughstandard for commercial resins, tells us little about their microstructures. Amore descriptive classification, based on their microstructural characteristics, ispresented in Figure 1.4.
HDPE and LLDPE are made with coordination catalysts, while LDPE is made withfree radical initiators. LDPE has both SCB and LCB, while polyethylenes made bycoordination polymerization generally have only SCBs. Some polyethylene resinsmade with specific metallocenes or Phillips catalysts may also have some LCBs,but their LCB topology is distinct from that of LDPE resins. Most commercialHDPE and LLDPE grades are made with Ziegler–Natta or Phillips catalyst. Phillipscatalysts are very important for the production of HDPE but are not used for LLDPEmanufacture. Metallocenes can be used in making both HDPE and LLDPE, butmetallocene resins are very different from the ones made with either Ziegler–Nattaor Phillips catalyst, as explained below. The market share of metallocene resins isstill relatively small but has been increasing steadily since the 1990s. Resins madewith late transition metal catalysts have had no significant commercial applicationsto date.
The mechanism of SCB and LCB formation in LDPE is different from that incoordination polymerization; in LDPE, LCBs are formed by transfer-to-polymerreactions, while SCBs result from backbiting reactions. Contrarily, SCBs in HDPEand LLDPE are produced by the copolymerization of α-olefins added to the reactor ascomonomers. LCBs, when present, are also formed by copolymerization reactions
6 1 Introduction to Polyolefins
Figure 1.5 Short-chain branch formation mechanism in coordination polymerization. Thechains are shown growing on a titanium active site.
with a polymer chain having a terminal group containing a reactive double bond(macromonomer).
Figure 1.5 illustrates the SCB formation mechanism during the copolymerizationof ethylene and α-olefins. The SCB behaves as a defect in the polymer chain,decreasing polymer density, crystallite size, and melting temperature. Therefore,the higher the molar fraction of α-olefin in the polymer chain, the lower itscrystallinity. HDPE resins have very low α-olefin comonomer fractions (typicallybelow a few mole percentage), while the comonomer content increases from LLDPEto ULDPE to VLDPE.
Density is, therefore, a reflection of the α-olefin molar fraction in the polyolefinchain, and it also depends, to a lower degree, on its molecular weight; all otherfactors being the same, polyolefins with higher molecular weight averages tend tohave a slightly lower density than those with lower molecular weight averages.
Density has been used for decades to classify polyethylene resins, but it is apoor descriptor for these materials because the microstructure of commercialpolyethylenes is too complex to be captured with a single density value. Let usfirst focus on the chemical composition distribution (CCD) of LLDPEs, that is, thedistribution of α-olefin fraction in the polymer chains. Most commercial LLDPEsare made with heterogeneous Ziegler–Natta catalysts. These catalysts have morethan one type of active site, each one producing polymer chains with differentaverage comonomer fractions and molecular weights. In addition, active sites thatfavor α-olefin incorporation also result in polymers with lower average molecularweights. As a consequence, the CCDs of Ziegler–Natta LLDPE resins are very
1.2 Polyethylene Resins 7
Increasing α-olefin percentage (SCB)
Figure 1.6 Generic chemical composition distribution of an LLDPE resin made with a het-erogeneous Ziegler–Natta catalyst.
broad, generally bimodal, and the average α-olefin content is correlated to thepolymer molecular weight, as illustrated in Figure 1.6.
Two distinct regions can be identified in Figure 1.6: a sharp high-crystallinity peak(low α-olefin fraction) and a broad low-crystallinity peak (high α-olefin fraction).These two regions are associated with at least two types of active sites, one withmuch lower reactivity ratio toward α-olefin incorporation than the other. As therelative amounts of polymer made under these two modes vary, polyethylene resinsvary from HDPE, with a unimodal, high-crystallinity peak and sometimes a small,lower-crystallinity tail, to MDPE, LLDPE, ULDPE, and VLDPE, with increasinglypronounced lower-crystallinity peak. The shape of the CCD is a strong function ofthe catalyst type, but it also depends on ethylene/α-olefin ratio, α-olefin type, andpolymerization temperature.
From the discussion of Figure 1.6, it is apparent that classifying these complexmicrostructures according to a single density value is inadequate. The picturebecomes even more complex when we take a look at the joint distribution of molec-ular weight and chemical composition (MWD × CCD) for Ziegler–Natta LLDPE,such as the one depicted in Figure 1.7. This tridimensional plot summarizes thecomplexity inherent to most commercial polyolefin resins. It also demonstrates thatmicrostructural characterization techniques are indispensable tools to understandthese polymers, as discussed in Chapter 2.
The MWD × CCD correlation exemplified in Figures 1.6 and 1.7 is not desirablefor certain polyolefin applications. A notable example are bimodal pipe resins, wherebetter mechanical properties are achieved if the higher molecular weight chainsalso have a higher α-olefin fraction than the lower molecular weight component.The reason for this improved performance has been linked to the presence oftie molecules, a subject that is, unfortunately, beyond the scope of this book. Thereader is directed to the references at the end of the chapter for more information on
8 1 Introduction to Polyolefins
α-Olefin mole percentage
Figure 1.7 Joint distribution of molecular weight and chemical composition (MWD ×CCD) for an LLDPE made with heterogeneous Ziegler–Natta catalysts.
Figure 1.8 Polyethylene with regular and reverse comonomer incorporation made in single-and dual-reactor systems, respectively.
this subject. The usual MWD × CCD correlation observed in polyethylene resinsmade with heterogeneous Ziegler–Natta catalysts can be partially reversed usingat least two reactors in series, as depicted in Figure 1.8. The polymers are calledbimodal polyethylenes because they have broad, and sometimes bimodal, molecularweight distribution (MWD). The first reactor makes low molecular weight HDPE inthe absence, or under very low concentration, of α-olefin. Hydrogen, the standardchain transfer agent in olefin polymerization, is used in the first reactor to lowerthe polymer molecular weight. The polymer made in the first reactor is thentransferred continuously to the second reactor, which is operated under higherα-olefin concentration in the absence, or under a much lower concentration, ofhydrogen, thus producing an LLDPE component with higher average molecular
1.2 Polyethylene Resins 9
1.2 mol% (replicate)
1-Hexene mole percentage
Figure 1.9 Chemical composition distributions of ethylene/1-hexene copolymers made witha metallocene catalyst.
weight than the HDPE component made in the first reactor. Many polyethyleneindustrial processes include two reactors in series to broaden the range of productproperties, as described in Chapter 4.
The advent of metallocene catalysts added a new dimension to commercialpolyolefin resins. Metallocenes are single-site catalysts that are used to makepolyethylenes with completely different microstructures from those made withZiegler–Natta and Phillips catalysts, but are still classified loosely as HDPE andLLDPE. Polyethylenes made with metallocene catalysts have uniform microstruc-tures, with narrow MWDs and CCDs. Figure 1.9 shows the CCDs for a seriesof ethylene/1-hexene copolymers made with a metallocene catalyst. All distri-butions are narrow and unimodal in sharp contrast to the behavior observedfor Ziegler–Natta LLDPEs. Notice the uniform incorporation of 1-hexene andthe absence of the high-crystallinity peak. In addition, their average copolymercomposition is independent of their MWD.
From a polymerization reaction engineering point of view, polyolefins madewith metallocene catalysts provide an excellent opportunity for model developmentbecause they have ‘‘well-behaved’’ microstructures. Chapter 6 shows that modelsdeveloped for single-site catalysts can also be extended to describe the morecomplex microstructures of polyolefins made with multiple-site complexes such asZiegler–Natta and Phillips catalysts.
Substantially linear polyethylenes are an important new class of polyolefins.These polymers are also made with single-site catalysts, but their main characteristicis the presence of LCBs formed by terminal branching. They are called substantiallylinear because their LCB frequencies are typically below a few LCBs per 1000carbon atoms. Terminal branching is illustrated in Figure 1.10, showing a polymer
10 1 Introduction to Polyolefins
CH 2 =
Figure 1.10 Long-chain branch formation through terminal branching promoted by asingle-site catalyst.
1 1.5 2 2.5 3 3.5 4 4.5 5
Figure 1.11 Model predictions for the long-chain branch and chain length (r) distributionsof substantially linear polyethylene.
chain with a reactive terminal bond being copolymerized with ethylene to forman LCB. The branching topology resulting from this mechanism is very differentfrom that of LDPE resins. Figure 1.11 illustrates a model prediction for thechain length distribution and LCB frequency for a polyolefin formed via thismechanism. More details on this LCB formation mechanism are provided inChapter 6.
Because propylene is an asymmetrical monomer, polypropylene can be pro-duced with different stereochemical configurations. The most common types ofpolypropylene, shown in Figure 1.12, are isotactic, syndiotactic, and atactic. In iso-tactic polypropylene, the methyl groups are placed on the same side of the backbone;in syndiotactic polypropylene, on alternating sides; and in atactic polypropylene,the methyl groups are arranged randomly along the chain. Atactic polypropylene
1.3 Polypropylene Resins 11
Figure 1.12 Main polypropylene types: (a) isotactic, (b) syndiotactic, and (c) atactic.
is amorphous and has little commercial value. Both isotactic and syndiotacticpolypropylene are semicrystalline polymers with high melting temperatures. Iso-tactic polypropylene dominates the market, likely because it is easily produced withheterogeneous Ziegler–Natta and metallocene catalysts; syndiotactic polypropy-lene can be produced only with some metallocene catalysts and has much lesswidespread commercial use.
Modern Ziegler–Natta catalysts used for propylene polymerization make isotacticpolypropylene with a very small fraction of atactic polypropylene. Non-specific sitesare responsible for the formation of atactic chains in Ziegler–Natta catalysts. Manyyears of catalyst development were required to minimize the fraction of thesecatalyst sites, as discussed in Chapter 3.
Ziegler–Natta catalysts also are used to make chains with very high regioregular-ity, favoring 1-2 insertions and head-to-tail enchainment (Figure 1.13). Defects suchas a 2-1 insertion following a 1-2 insertion create irregularities along the polymerchain, decreasing its crystallinity and melting temperature. Several metallocenecatalysts produce polypropylene with very high isotacticity but lower regioregular-ity, which causes their melting temperatures to be lower than of those made withZiegler–Natta catalysts. Metallocene catalysts can also make polypropylenes withother stereostructures such as atactic–isotactic block chains, but these productshave not found commercial applications yet.
Impact propylene/ethylene copolymers4) are produced using at least two re-actors in series with heterogeneous Ziegler–Natta catalysts or supported metal-locenes. The first reactor makes isotactic polypropylene, and the second producespropylene–ethylene random copolymer. The copolymer component is amorphousor has very low crystallinity, and is intimately dispersed in the homopolymerphase, even though the two phases are immiscible. The copolymer phase dissipates
4) These materials are sometimes (erro-neously) called block copolymers. In fact,they are heterophasic materials composed
of isotactic polypropylene and randompropylene/ethylene copolymer chains.
12 1 Introduction to Polyolefins
Head to tail
Head to head
Tail to tail
Figure 1.13 Regioregularity in polypropylene polymerization.
Polypropylene matrix (top reactor)
E/P Rubber domains (bottom reactor)
High impact PP
25 μm0 μm
Figure 1.14 Process for the production of impact polypropylene.
energy during impact, greatly increasing the impact resistance of these resins.Several processes have been designed to produce impact polypropylene of highquality, as discussed in Chapter 4. Figure 1.14 schematically illustrates a processfor the production of impact polypropylene.
Finally, the same comments made for Ziegler–Natta versus metallocene polyethy-lene apply to polypropylene resins. Metallocene catalysts make polypropylene withnarrower MWD and, in the case of copolymers, narrower CCD.
Further Reading 13
There are several excellent books onpolyethylene and polypropylene proper-ties and applications. The Handbook ofPolyethylene is a good source of informa-tion on HDPE, LLDPE, and LDPE.
Peacock, A.J. (2000) Handbook of Polyethylene,Marcel Dekker, New York.
Two multiauthored books on polypropyleneare also recommended.
Karian, H.G. (ed.) (2003) Handbook ofPolypropylene and Polypropylene Composites,Marcel Dekker, New York.Karger-Kocsis,J. (ed.) (1999) Polypropylene. An A-Z Ref-erence, Kluwer Academic Publishers,Dordrecht.
The Encyclopedia of Polymer Science andTechnology has excellent entries on HDPE(Benham, E. and McDaniel, M. (2002)Ethylene polymers, HDPE, in Encyclopediaof Polymer Science and Technology (ed. H.F.Mark), John Wiley & Sons, New York.doi: 10.1002/0471440264.pst408.pub2),LDPE (Maraschin, N. (2002) Ethylenepolymers, LDPE, in Encyclopedia of Poly-mer Science and Technology (ed. H.F.Mark), John Wiley & Sons, New York.doi: 10.1002/0471440264.pst121), LLDPE(Simpson, D.M. and Vaughan, G.A. (2002)Ethylene polymers, LLDPE, in Encyclo-pedia of Polymer Science and Technology
(ed. H.F. Mark), John Wiley & Sons, NewYork. doi: 10.1002/0471440264.pst122),ethylene/propylene elastomers (Noorde-meer, J.W.M. (2002) Ethylene-propyleneelastomers, in Encyclopedia of Poly-mer Science and Technology (ed. H.F.Mark), John Wiley & Sons, New York.doi: 10.1002/0471440264.pst125), andpolypropylene.
Steward, C. (2002) Propylene polymers, inEncyclopedia of Polymer Science and Tech-nology (ed. H.F. Mark) John Wiley & Sons,New York. doi: 10.1002/0471440264.pst301
These references are constantly updated bythe authors and can be accessed on-line,making them a valuable source of infor-mation on these polymers.
We have also published general overviewson olefin polymerization reaction en-gineering, covering polymerizationmechanisms and catalysis, properties,characterization, and mathematicalmodeling.
Soares, J.B.P. and Simon, L.C. (2005) Coor-dination polymerization, in Handbook ofPolymer Reaction Engineering (eds T. Meyerand J. Keurentjes), Wiley-VCH, Weinheim,pp. 365–430.Soares, J.B.P., McKenna, T.F.,and Cheng, C.P. (2007) Coordination poly-merization, in Polymer Reaction Engineering(ed. J.M. Asua), Blackwell Publishing,pp. 29–117.